Pré-visualização7 páginas

Basic ideas behind the modelling Below is a summary of some of the thinking behind the development of the model. To sustain process variations and obtain desirable chemistry conditions it is necessary to have the right and homogenous temperature at the inlet, near the slag and at the outlet. The regions of homogeneity should be as large as possible. The temperature field is strongly in- fluenced by the velocity field. Near the outlet, the veloc- ity field has to be as vertical and symmetric as possible to prevent clogging. Near the steel/slag interface, the transport should be almost horizontal and calm. This can be attained by using flow guides to redesign the flow field. The consideration of refractory, slag and flux makes it possible to do conjugate heat-transfer calculations right out to the surfaces. Heat conducted to the outermost surface can be heat-exchanged to the surroundings. This is modelled by using temperature-dependent radiative and convective boundary conditions resulting in a phys- ically more correct solution. Solidification at cold parts of the innermost surfaces can be considered in the mod- els. Refractory surfaces suffering from erosion and/or dissolution might be taken into account. Including the refractory in the calculation would also be advantageous in that it would make it possible to use IR techniques for some validation purposes. The mixing of slag and metal in a zone where the velocities are low is thought to originate from the 16 Investigation of slag floatation and entrapment instability that arises when 2 streams of fluid, with sta- ble density differences, flow past one another. The pres- ence of shear leads to instability, which is characterised by the growth of waves, later rolling up into (small) vortices. This shear instability, ‘The Kelvin–Helmholtz Instability’, may serve as the mechanism of mixing be- tween the layers, promoting the vertical transport of properties such as heat or reactants. Furthermore, Spald- ing & Villasenor [16] have shown by using a long duct of a rectangular cross section and 2 fluids of different densities, that this instability could be predicted with a fluid-flow calculation if the position of the interface was calculated. Using these ideas as the basis for the mod- elling approach, a mathematical model of continuous- casting tundish could be extended to include the slag phase. This development enables predictions of fluid- flow and heat-transfer conditions in the highly impor- tant steel/slag region. Conservation equations The model is steady or unsteady and is based on con- servation equations for the following: Conservation of mass ∂ρ ∂t + ∇ · (ρ �V) = 0, (1) where ρ is density and �V is velocity. Conservation of momentum ρ · D �V Dt = −∇P + �B + µ · ∇2 �V, (2) where P is pressure, B is volume force and µ is dynamic viscosity. Conservation of energy ρ · De Dt − ∇ · k∇T − ∇ · (∑ j ρDj · e j · ∇m j ) − µ · � − DP Dt − S = 0, (3) where e is the static enthalpy, k is the thermal conduc- tivity, T the absolute temperature, µ is the dynamic vis- cosity, S is the source function (i.e. the thermal energy created per unit volume) and � = ( ∂ui ∂xj + ∂u j ∂xi − 2 3 ∂u1 ∂x1 δi j ) ∂ui ∂xj is the dissipation function. The first and last term in the dissipation function within the brackets come from the viscous part of the normal stresses, whereas the second term comes from the shear stresses. Conservation of elements in each phase ρ · �V · Dnα Dt = ∇ · (∑ j ρDj · nα, j · ∇m j ) , (4) where nα is the mass fraction of element α in mixture of compounds, Dj is the mass diffusion coefficient for component j, nα,j is the mass fraction of element α in a compound substance j and mj is the mass fraction (con- centration) of substance j in mixture. Turbulent transport equations. The LVEL algebraic tur- bulence model is a unique feature (built into PHOEN- ICS) useful for conjugate-heat-transfer problems. Far away from the wall, it reduces to the well-established result [18]: v+ = K · y+, (5) where v+ is the dimensionless effective viscosity, K is the von Karman constant (0.417) and y+ is the dimensionless distance from the wall. Auxiliary equations Property variations of the steel phase Density. The temperature-dependent density of steel is described by the following expression [19]: ρl = 8.586 · 103 − 0.8567Tl, (6) where Tl is the temperature of the steel. Heat capacity. The temperature-dependent heat capac- ity is calculated as [20] C p,Fe = ( 452.963 + 176.704 · 10−3Tl − 482.082 · 10 5 T2l ) . (7) Dynamic viscosity. The temperature-dependent dy- namic viscosity is calculated as [19] µl,l = 0.3147 · 10−3 exp ( 46480 8.3144Tl ) , (8) where Tl is the temperature of the steel. Property variations of the liquid slag phase The following typical slag composition was chosen for the calculations: 50% CaO, 12.5% Al2O3, 7.5% MgO and 30% SiO2. Heat capacity. The temperature-dependent heat capac- ity for slag is calculated as [21] C p,CaO = 4.1868 · 10 3 56.079 ( 11.86 + 1.08 · 10−3Ts − 1.66 · 10 5 T2s ) , (9) 17 Solhed & Jonsson C p,Al2O3 = 4.1868 · 103 101.961 ( 28.804 + 2.197 · 10−3Ts − 11.56 · 10 5 T2s ) , (10) C p,SiO2 = 4.1868 · 103 60.084 ( 17.119 + 0.452 · 10−3Ts − 9.335 · 10 5 T2s ) , (11) C p,MgO = 4.1868 · 10 3 40.304 ( 11.707 + 0.751 · 10−3Ts − 2.734 · 10 5 T2s ) , (12) Cps = (%CaO)C p,CaO + (%Al2O3)C p,Al2O3 + (%MgO)C p,MgO + (%SiO2)C p,SiO2 , (13) where Ts is the temperature of the slag. Dynamic viscosity. The temperature dependence of the dynamic viscosity for the slag is given by the following expression [22]: µl,s = 1.0 · exp ( −5.589 + 24323.7 Ts − 0.7099 · ln(Ts) ) (14) where Ts is slag temperature. Treatment of the liquid slag phase General equations. Incorporation of the slag phase into the model of the tundish has been carried out by using the following 2 equations [23–26]: ∂ ∂t (ρlcl) + div(ρl �Vlcl) = 0, (15) ∂ ∂t (ρscs) + div(ρs �Vscs) = 0, (16) where �Vl is the velocity vector for the steel phase and �Vs is the velocity for the slag phase. The variable cl has, at time 0, the value 1 in the regions where there is only steel and has the value 0 in the regions where initially there is only slag. Similarly, cs has the values 0 and 1 in the regions where the tundish initially contains only steel and slag, respectively. The volume of steel per unit mass, Vst, and the volume of slag per unit mass, Vsl, are calculated as follows [23]: Vst = clcl + cs 1 ρst , (17) Vsl = cscl + cs 1 ρsl , (18) where ρsl is the density of the slag and ρst is the density of steel. The total volume of the liquid phase (steel and slag) per unit mass is given by [23] Vtot = Vst + Vsl. (19) Treatment of the solid slag phase (flux). The computa- tional area where covering powder blocks the flow is set to have the following physical properties [27]: density 600 kg/m3 specific heat 1180 J/kg ◦K thermal conductivity 1.7 W/m ◦K hermal expansion 0 Boundary conditions The most decisive boundary conditions for a solution are given below. The fixed mass flow at the inlet. The mass flux at the inlet is the product of the velocity (m/s) and the density (kg/m3) usually set in the first cell layer. The constant pressure at the outlet. At the outlet, the de- sired pressure normally is the dynamic pressure. There- fore it is convenient to set the reference pressure to 0. The frictional flow near the lining. At the fluid/solid in- terfaces fully developed friction is set. The emissivities and heat-transfer coefficients for slag and tundish surfaces. The heat transfer takes part both through the lining and through the flux. The lin- ing is usually 4-layered and results in the following expression: θs − θg = 1k · φ A 1 k = 1 αs + n∑ 1 δi λi + 1 αg (20) where θx is temperature at different layers (s is steel, g is surrounding gas), k is heat transmission coefficient, αs and αg are heat-transfer coefficients at steel-refractory and outer surfaces respectively (W/m2